During the last decade magnesium and magnesium alloys (MA) were the centre of a large number of studies especially in Europe [1-3] and Asia [4-6]. The main focus of these studies was to evaluate the use of magnesium and MA as basic material for clinical applications.
For the treatment of bone fractures, orthopaedic implants made of surgical steel or titanium are used when weight bearing bones are affected. The major disadvantage of these materials is that they need to be removed in a second surgery due to implant loosening or intolerance after longer implantation times resulting in higher costs and stress for the patient. Therefore resorbable implant materials are needed which complementarily provide sufficient stability for weight bearing applications.
Magnesium is a light metal which is known to corrode in aqueous solution. Its density is 1.74 g/cm3 at room temperature and therewith 1.6 fold resp. 4.5 fold lower than aluminium or steel . With prospect of orthopaedic use, its advantages are its appropriate compressive and tensile strengths as well as its Young’s Modulus (41-45 GPa), which is considerably closer to cortical bone compared to other metallic implant materials [7-9]. The corrosion rate ranges between aluminium and unalloyed steel .
Magnesium as a mineral occurs naturally in the body and is eliminated through the kidneys [11,12]. Due to their high excretion ability hypermagnesaemia is rare . Severe symptoms like arrhythmia, feeling of faintness up to paralyses and/or cardiac or respiratory arrest are only seen in the course of therapeutical intravenous application [11,14].
Therefore, magnesium and MA are intensively investigated to develop a basic material for the production of degradable osteosynthesis implants e.g. plates, screws or intramedullary nails.
Alloying with other elements such as lithium, aluminium, zinc or rare earth metals aims to adjust the corrosion resistance and mechanical properties of magnesium [9,15-18]. In engineering applications
The main reason for the addition of
The usual addition of
There are controversial reports about the effect and toxicity of REs. Especially high concentrations are considered to have toxic effects [42-45].On the other hand a bone-protective effect and an increase in bone density could be shown after a six months feeding trial . Low amounts of REs in MA were appraised as well tolerable in reference . In reference  the short-term effect of REs in vitro was evaluated. The authors assessed the responses of different cell lines after the addition of the single RE elements and found differences between light (Lanthanum (La), Cerium (Ce), Praseodymium (Pr)) and medium to heavy (Neodymium (Nd), Europium (Eu), Gadolinium (Ga) and Dysprosium (Dy)) RE elements: light RE elements showed toxic effects at lower concentrations . They concluded that La and Ce should be used only when absolutely necessary. Most of the contemporarily published in vivo examinations used MA with low amounts of REs, which were added as mischmetal [2,9,40,47-50]. This mischmetal can actually differ depending on the time and/or date of purchase. For example,  determined the RE mixture of WE43 to be mainly Nd, Gd and Dy whereas in the most commercially available RE composition metals Ce, Nd and La form the major fraction [44,51]. In
But despite the good results of LAE442, the effort to replace the mixture by a single element is still reasonable to achieve a most accurate implant device.
Since in reference  Nd was classified as suitable, referring to LAE442, LANd442 was developed as well as Nd2 and their in vitro corrosion behaviour was assessed . They showed that the corrosion rate for Nd2 was lower than for LANd442. However, the application of a MgF2-coating lowered the corrosion rate of LANd442. After these positive results, LANd442 was introduced into in vivo experiments. Parts of this study will be included in the next subchapter.
Some groups reported on the fact that in vitro and in vivo degradation properties could differ considerably [6,24]. Thus, besides profound in vitro tests like bending tests, corrosion tests or microstructure characterisation to identify and adjust the material properties, the in vivo degradation behaviour and biocompatibility has to be investigated thoroughly.
To investigate the clinical applicability of different RE containing MA the rabbit (female New Zealand White rabbits, body weight > 3 kg) was chosen as animal model. Partially, the results of the following data have already been published or submitted [55-57]. Extruded, cylindrical pins (length 25 mm, diameter 2.5 mm) were produced and washed in acetone for eliminating fabrication residues. Sterilization was carried out by gamma irradiation. Ten implants of three different RE containing MA were produced: LAE442, LANd442 and ZEK100. These cylinders were randomly implanted into the middle third of the tibial medullary cavity (Fig 1), one in each hind leg. The follow up period was six months. Clinical examinations were performed regularly to assess the clinical tolerance of the implants.
µ-Computed tomography is a non-destructive analysing method to assess changes within the structure of either engineering components or medical implants [2,40,58,59]. It can also be used to evaluate the reactions of the surrounding tissue to implanted orthopaedic devices after in vivo examinations [57,60,61]. However, the laboratory animals have to be sacrificed for these investigations. To evaluate the proceeding degradation and to perform a proper initial-to-end-value comparison in vivo µ-computed tomography scans have been introduced recently [50,55,57,60,62]. Further they allow for a reduction of laboratory animals as the results after different implantation periods could be gained from the same animal.
For the presented study an XtremeCT (Fa. Scanco Medical, Zurich, Switzerland) was used. The animals were scanned in general anaesthesia and in supine position (Fig.2). The scan was performed from the knee joint space up to approx. 5 mm beneath the implant (Fig.1) with a resolution of 41 µm, 1000 projections at 0-180° and an integration time of 100 ms. The electron energy used was 60 kVp and the intensity was 900 µA. In the first eight weeks the rabbits were scanned biweekly, afterwards every four weeks.
The µ-computed tomography evaluation
Second the gas which emerged during the degradation process of magnesium implants was assessed. The corrosion mechanism of pure Mg and MA consists of two electrochemical parts: the anodic partial reaction forms Mg2+ and 2e-, whereas the cathodic partial reaction evolves hydrogen and 2OH- from the reaction of water with the 2e- [10,63,64]. In vitro corrosion tests of MA which quantify the amount of emerging gas utilize this mechanism . Many in vivo studies reported on the emergence of gas during the course of MA-implant degradation either as diffuse accumulation or palpable and non-palpable gas bubbles underneath the skin [23,55,58,65]. It is a continuous discussion, if these bubbles actually contain hydrogen. Hence, as a supplementary investigation a gas-tight syringe was used to gather the emerged gas (approx. 0.5 ml) out of a large subcutaneous gas bubble. It was sent to the Institute of Organic Chemistry, Technical University Braunschweig, and analyzed. However, it was not possible to verify pure hydrogen. The most likely explanation is that the highly volatile gas undergoes rapid exchange with the surrounding tissue. From the authors’ point of view there is no need to doubt that the degrading magnesium implants are the source of the gas independent on the actual composition in the bubbles as faster degrading alloys subjectively generate higher amounts of gas. This leads to the matter of quantifying the gas volume. So far, no method has been described to report on the quantity of gas emerged particularly over the course of time. So within this second part of the µCT evaluation a method for quantifying the gas volume using the XtremeCT was established. Within the 2D-slices of the µCT-scans of the LAE442 group, the occurring gas was manually outlined and measured by means of the software µCT evaluation program V6.1. The threshold of the grey values was determined to be between -1000 and 25.
With proceeding degradation the corrosion products influence the surrounding tissue. The smaller the impact of the implant the better is its biocompatibility. On the one hand it could be generally said, that an implant is biocompatible when its functionality is achieved without inducing a foreign body reaction . On the other hand, according to the Conference 1984 of the European Society for Biomaterials, biocompatibility is the ability of a material to fulfil its purpose for a specific application with an appropriate host response . This definition includes the fact that every inserted implant actually could/will influence the surrounding tissue in one or another way and emphasize on the adequacy. The reactions which are described are either foreign body reactions ([3,57,60,65] or structural changes of the bone [2,57,61]. To assess cellular reactions histological examinations have to be carried out. However, µCT is a well-established tool to evaluate structural changes of the bone. Thus, as a third part of the µCT evaluation the impact of the degrading implant on the adjacent bone was evaluated by a quantitative determination of the bone density (in mg HA/cm3), the bone volume (in mm³/slice) and the bone porosity (in percent). The bone volume which was included into the evaluation was defined by choosing those slices in which also the implant was seen. Hence, the bone directly adjacent to the implant was manually outlined. The threshold value for the subsequent evaluations was determined to be 160 and the same software was used as for the implant and gas evaluation. Due to internal processing, the latest investigation time for ZEK100 was week 20.
2.1. Pin degradation
The density is given in the unit mg HA/mm³ (milligram hydroxyapatite per cubic millimetre) which is the unit the XtremeCT gives for the density of mineralized tissue such as bone. Therefore, the indicated density values do not correspond to common used alloy density values but allow for a comparison of the three alloys investigated among each other. Their density differed from the beginning of the implantation period. LAE442 density was higher than LANd442. ZEK100 showed the lowest density (Fig. 3). Besides the varying alloying components different grain sizes of the alloy could influence the density  and therefore cause the detected differences. During the course of degradation LAE442 showed only a slight decrease in density with a very low standard deviation. Also the density of LANd442 implants diminished slightly, however the standard deviation was obviously higher implying a more inhomogeneous procedure. ZEK100 implants showed the highest loss in density.
The initial volume of all alloys ranged in similar values. According to the density, LAE442 implants showed only a minor decrease over the implantation period and demonstrated again a low standard deviation. The changes of volume in LANd442 implants also matched the results of the density. A slight decrease could be found with a higher standard deviation in comparison to LAE442. ZEK100 pins demonstrated an obvious loss of volume particularly from the 12th week on with an exceptional high standard deviation in the later scan weeks (Fig. 3).
These results indicate a slow and uniform degradation of LAE442 implants. LANd442 pins also degraded slowly but less uniformly. ZEK100 showed an equally slow degradation within the first weeks of implantation. This process accelerated distinctly resulting in inhomogeneous pin geometries.
The examination of the true 3D-thickness confirmed these findings (Fig. 4). Corresponding to the volume and density changes, the average diameter of the spheres and thus the true 3D-thickness of LAE442 implants underlay only minor changes in the course of degradation. The low and uniform variance of diameter is a sign for a very homogeneous degradation. LANd442 implants showed a slight decrease of the true 3D-thickness. The variance of diameter increased in the course of implantation moderately. Taken together both results it could be said that LANd442 pins degraded slowly but faster and more inhomogeneous than LAE442. ZEK100 displayed the most obvious changes. From the 8th week on the average diameter of the spheres decreased continuously while the variance of diameters showed a profound increase. Consequently, ZEK100 implants degraded fast and irregularly.
The colour mapping of the degraded implants after six months implantation duration in comparison to an undegraded implant visualized the differences of the pin geometry (Fig. 5).
2.2. Gas volume
In outlining and evaluating the occurring gas within the marrow cavity it was possible to quantify the gas volume during the course of degradation.
It is noteworthy that a distinct proceeding decrease in volume was found until week 12 followed by a continuous increase. This could be explained by the fact that a certain amount of gas was brought into the marrow cavity due to the surgical procedure. This gas volume is reabsorbed by the organism in the subsequent time. Corresponding to the beginning degradation of the implant, which is represented by the volume and density changes (Fig. 6 and 7), the amount of gas which is emerged exceeded the absorption capacity of the organism resulting in the increase of gas volume.
Fig. 8 shows a 3D-evaluation of the bone (transparent) with implanted MA-cylinder (blue) and surrounding gas (brown).
For further examinations, this method can be used to compare the gas volume with possible occurring changes of the surrounding tissue.
2.3. Changes in bone structure
The bone adjacent to all three types of implanted MA pins lost density during the course of degradation (Fig. 9). For LAE442 implants the decrease in density was more pronounced in the first weeks of implantation and slowed down in the following period. From week 12 on only a negligible further decrease could be seen. LANd442 also showed a moderate decrease in bone density up to week 12 followed by an increase in the next four weeks and subsequent steady state until week 24. Due to the lower number of investigations the density course of ZEK100 implants appeared to be different. They induced a proceeding reduction of the bone density over the total investigation period. However, a higher number of investigations could reveal a similar pattern as for LAE442 and LANd442.
The bone volume (specified per slice) increased over the investigated time period.
No distinct differences could be found for the different MA cylinders (Fig. 10).
In contrast to the aforementioned results the changes in porosity of the bone showed no regular pattern (Fig. 11). The bone porosity adjacent to LAE442 implants first increased up to week 4, followed by a decrease up to week 12. Afterwards the bone porosity again increased up to the end of the investigation period but slower than in the beginning. LANd442 implants showed only minor changes within the first 12 weeks. After that the porosity increased first moderately up to week 16 and from then on intensely till the end of investigation. However this increase in the LANd442 mean value is particularly caused by one implant which degraded severely faster than all other implants of the same group without any obvious explanation. The high standard deviation for the scans in week 16 and 24 illustrated this fact. If this cylinder would be excluded from the evaluation the mean porosity of the LANd442 pins would steadily decrease from week 8 on up to week 24. After the implantation of ZEK100 cylinders a distinct increase in bone porosity could be seen in the first eight weeks followed by a moderate decrease up to week 20.
Taken into account all gathered results the µ-computed tomography evaluation of the bone structure illustrated the bone remodelling processes well. The increase in bone volume indicated endosteal and periosteal new bone growth. The simultaneous decrease in bone density can be explained by the fact that this newly formed bone is not as dense as the mature bone. The varying porosity depends on two different factors. On the one hand the state of the bone remodelling process influences this value. The newly formed bone is not as much structured as the mature bone and therefore shows a higher porosity. Since the bone of LAE442 implants showed a higher increase in bone volume accompanied by the most distinct decrease in density particularly in the first weeks of implantation the ascending porosity at this time could be explained. On the other hand the two-dimensional evaluation which was not included here showed that the faster degrading ZEK100 implants induced more bone cavities than the slower degrading alloys . This is probably the cause for the initial increase in porosity. To which extend the decreasing density influences the computation of the porosity remains to be shown as the further degrading ZEK100 cylinders should continuously increase the porosity instead of the determined however slight decrease.
After considering both the accessible literature and the presented results, REs seem useful and maybe even necessary alloying components in MA basis material for the production of orthopaedic implants.
It could be shown that the addition of REs lead to mostly biocompatible, degradable implants with however different degradation characteristics.
LAE442 proved to be the slowest degrading alloy with the lowest influence on the surrounding tissue. The replacement of the RE composition metal by the single element Nd did not result in improvement of the biocompatibility nor of the degradation behaviour. Contrary, these LANd442 implants showed a less regular corrosion process than LAE442 cylinders. Therefore LAE442 implants should be favoured over LANd442. Therewith, two alloys which aimed to replace the RE composition by a single element (LANd442, LACe442 ) failed in exceeding the good degradation behaviour and biocompatibility of LAE442.
ZEK100 as a completely different approach to develop an alloy for orthopaedic implant production clearly showed inferior results by degrading inhomogeneously and causing significant structural changes in the adjacent bone and tissue .
In principal, a slow degrading MA should be developed as a faster degradation is correlated with a reduced clinical tolerance and an increased impact on the adjacent bone: the implant in the right leg of one LANd442 rabbit degraded significantly faster than the other implants. The animal showed a moderate to severe lameness of the affected leg and an obvious increase in bone porosity. Also in reference was reported on the poor biocompatibility of LACer442 which degraded very fast.
Altogether, the perfect composition of a degradable MA implant material has not been developed yet. Regarding the biocompatibility, Li-Al-RE-containing MA turned out to be very promising. However, to satisfy the high standards for the production of medical devices efforts to replace the RE composition metal by one or even a couple of the single RE elements should not be abandoned with further focus on a slow and homogenous degradation behaviour.
The authors thank Dr. Ulli Papke from the Institute of Organic Chemistry (TU Braunschweig) for analyzing the gas out of the gas-tight syringe.
The presented results are part of the collaborative research centre (CRC599, Medical University of Hannover, University of Veterinary Medicine Hannover and University of Hannover), which is sponsored by the German Research Foundation (DFG).